- Hot search：
ISO 4895-2014 pdf free download
ISO 4895-2014 pdf free download.Plastics — Liquid epoxy resins— Determination of tendency to crystallize
Plastiques — Résines époxydes liquides — Determination de Ia tendance a Ia cristallisation.
2 Normative references
The following documents, in whole or in part, are normatively referenced in this document and are indispensable for its application. For dated references, only the edition cited applies. For undated references, the latest edition of the referenced document (including any amendments) applies.
ISO 6353-2:1983, Reagents for chemical analysis — Part 2: Specfications — First series
ISO 6353-3:1987, Reagents for chemical analysis — Part 3: Specifications — Second series
Calcium carbonate powder is mixed with the liquid epoxy resin dissolved in ethanol, The mixture is kept at a specified low temperature and observed at specified time intervals to compare the changes in fluidity and crystallization.
4.1 Calcium carbonate as specified in ISO 6353-3:1987, R 53.
4.2 Ethanot.asspecilied in ISO 6353-2:1983,R 11.
5.1 RefrIgerator or cold enclosure, maintained at (10 ± 2) °C.
5.2 Glass test tube, of capacity approximately 100 ml, 40 mm in diameter and 80 mm in height, with a polyethylene-covered stopper.
5.3 Glass rod, of hard glass, approximately 10 mm in diameter.
5.5 Analytical balance, accurate to 0,01g.
5.6 Constant temperature room maintained at (23 ± 5)°C.
6.1 Weigh 20 gof liquid epoxy resin into the test tube (2).
6.2 Stopper the test tube and place it in the oven (5A) at (60 ± 2) °C for 16 h.
6.3 Cool the test tube to room temperature 1(23 ± 5) CI in the constant temperature room (J aud
20 g of calcium carbonate (4d) and 2 g of ethanol (42). and mix the sample thoroughly with the glass rod
6.4 Stopper the test tube again and place it In the vertical position in the refrigerator or cold enclosure (5,J) at (10 ± 2) °C.
6.5 Observe the sample twice a day at a specified time (for example at an interval of 8 h during the day
and 16 h during the night):
— to carry out first observation at 5 pm;
— to carry out second observation at 9 am (next day);
— to carry out third observation at 5 pm (next day);
— to carry out fourth observation at 9 am (the day after).
Observe the sample in the following way.
Allow the test tube to warm to room temperature 1(23 ± 5) °CJ in the constant temperature room (5J). then place it in the horizontal position and leave it for 1 mm.
— When the distance of movement of the liquid surface tip (L in Figure 1) is 10 mm and more, record a.
— When the distance of movement of the liquid surface tip (L in Figure 1) is less than 10 mm, record b.
— When the sample has completely solidified due to crystallization, record ‘c”.ISO 4895-2014 pdf free download.
All resources on this website are from the Internet. It is only for personal study and research. No one is allowed to use it for any commercial purpose. If you need, please buy the genuine standard. If there is any infringement of your copyright, please contact the webmaster in time, and I will correct it immediately.
- Maybe you like
- Latest Updates
- ISO 287-2009 pdf free download
- ISO 527-5-2009 pdf free download
- ISO 659-2009 pdf free download
- ISO 660-2009 pdf free download
- ISO 712-2009 pdf free download
- ISO 725-2009 pdf free download
- ISO 730-2009 pdf free download
- ISO 927-2009 pdf free download
- ISO 2041-2009 pdf free download
- ISO 3040-2009 pdf free download
- ISO 3506-2-2009 pdf free download
- ISO 3506-3-2009 pdf free download